O R I G I N A L P A P E R
Experimental investigation and thermodynamic modeling
of the Au–Ge–Ni system
Shan Jin•Liliana I. Duarte•Guoxing Huang •
Received: 18 February 2012 / Accepted: 15 April 2012 Ó Springer-Verlag 2012
Abstract Phase equilibria in the Au–Ge–Ni ternary sys-tem were studied by means of scanning electron microscopy, electron probe microanalysis, X-ray diffrac-tion, and differential scanning calorimetry. The phase relations in the solid state at 600°C as well as a vertical section at Au72Ge28–Ni were established. No ternary
compound was found at 600°C. On the basis of the experimental phase equilibria data, a thermodynamic model of the Au–Ge–Ni ternary system was developed using the CALPHAD method. Thermodynamically calcu-lated phase diagrams are shown at 600°C, in two vertical sections and the liquidus projection. Reasonable agreement between the calculations and the experimental results was achieved.
Keywords Au–Ge–Ni Thermodynamic Phase diagram CALPHAD
High Pb content alloys which contain as much as 85 wt.% Pb have been widely used in the electronic and automotive industries as soldering materials for high temperature application. Given the potential environmental impact of based alloys, the development of high temperature Pb-free solders has become very urgent. Possible candidates are Zn-based alloys (Zn–Al, Zn–Sn) [1,2], Bi-based alloys (Bi–Ag) , Sn–Sb based alloys , and especially Au-based alloys [5–8]. For example, Au–Si, Au–Sb, and Au– Ge alloy systems are all simple eutectic systems with low eutectic temperatures between 280 and 365°C . In addition to the low melting point, Au-based alloys also possess good thermal and electrical conductivity, excellent resistance to corrosion, high mechanical properties, etc. . Among various Au-based alloys, Au–Ge-based alloys are very attractive as possible high temperature Pb-free solders because of their good wettability and high bonding strength with the substrate materials (e.g., Cu and Ni) [11,
12]. In order to better understand the interaction mecha-nism of the Au–Ge solders with the normally used substrate Ni to facilitate solder design and processing optimization, phase equilibria and thermodynamic proper-ties of the Au–Ge–Ni system are indispensable.
Besides, Au–Ge or Au–Ge–Ni alloys have also been extensively used in ohmic contacts to GaAs semiconduc-tors [13,14]. Knowledge of the Au–Ge–Ni ternary system is also very important for their application in the semi-conductor industry.
However, the available information on the Au–Ge–Ni ternary system is rather scarce. Jaffee and Gonser  studied the additions of Ni up to 12.2 at.% into the Au–Ge alloys by metallography, thermal analysis, and X-ray dif-fraction and reported that Ni has little effect on the Au–Ge
Dedicated to Professor Herbert Ipser on the occasion of his 65th birthday.
S. Jin L. I. Duarte C. Leinenbach (&)
Laboratory for Joining Technologies and Corrosion, Empa, Swiss Federal Laboratories for Materials Science and Technology, U¨ berlandstrasse 129, 8600 Du¨bendorf, Switzerland
e-mail: firstname.lastname@example.org S. Jin
Computational Materials Laboratory, Ecole Polytechnique Fe´de´rale de Lausanne, Station 12, 1015 Lausanne, Switzerland G. Huang
School of Material Science and Engineering, Central South University, Changsha 410083, Hunan, People’s Republic of China
eutectic temperature. The freezing point of the eutectic line is lowered by Ni. In addition, they proposed that a ternary eutectic may occur in the Au–Ge–Ni ternary system. Christou  quoted a ternary eutectic temperature of 425°C and stated that it was determined by a resistivity technique.
Therefore, the objectives of the present work were (1) to study the phase relations of the Au–Ge–Ni ternary system, including an isothermal section at 600°C and a vertical section at Au72Ge28–Ni and liquidus projection; and (2) to
develop the thermodynamic description of the Au–Ge–Ni ternary system using the CALPHAD (CALculation of PHAse Diagram) method .
In the present optimization, the thermodynamic parameters of the Au–Ge, Au–Ni, and Ge–Ni binary subsystems are taken from , , and , respectively.
The pure elements in their stable structures at 298.15 K and 1 bar are chosen as the reference states for the system. The thermodynamic functions of the pure elements in their stable and metastable states are taken from the Scientific Group Thermodata Europe (SGTE) database  and are described as 0 GuiðTÞ ¼ GuiðTÞ H SER i ¼ a þ bT þ cT ln T þ dT 2 þ eT3þ fT1þ gT7þ hT9 ð1Þ where HSERi is the molar enthalpy of the element i (i = Au, Ge, or Ni) at 298.15 K and 1 bar in its standard element reference (SER) state; T is the absolute temperature; GuiðTÞ is the absolute molar Gibbs energy of the element i with structure of u;0GuiðTÞ is the molar Gibbs energy of the element i with the structure of u referred to the enthalpy of its stable state at 298.15 K and 1 bar.
The solution phase u (u = liquid, fcc, and diamond) is treated as a substitutional solution. Its molar Gibbs energy is expressed as Gum¼ xAu0Gu Auþ xGe 0Gu Geþ xNi 0Gu Niþ RTðxAuln xAu þ xGeln xGeþ xNiln xNiÞ þEGumþmagGum ð2Þ where Gumis the molar Gibbs energy of a solution phase u; 0Gu
i is the molar Gibbs energy of the element i (i = Au, Ge, or Ni) with the structure u in a nonmagnetic state; xi
the mole fraction of component i, R gas constant, T
m the excess Gibbs energy, and magGu
m is the magnetic contribution to the Gibbs energy. The excess Gibbs energy of phase u can be expressed by the Redlich– Kister polynomial  as EGu m¼ xAuxGeL u Au;Geþ xAuxNiL u Au;Niþ xGexNiL u Ge;Ni þ xAuxGexNiLuAu;Ge;Ni ð3Þ
here LuAu;Ge, LuAu;Ni, and LuGe;Niare the interaction parameters taken from the corresponding binary systems [18–20]. LuA;B¼X n j¼0 ðjÞLu A;BðxA xBÞ j ð4Þ
where ðjÞLuA;B¼ Ajþ BjTþ CjT ln T, and Aj, Bj, and Cj
are model parameters evaluated from experimental information. LuAu;Ge;Ni is the ternary interaction parameter with the following form:
LuAu;Ge;Ni ¼ xAu0Lu Au;Ge;Niþ xGe 1Lu Au;Ge;Niþ xNi 2Lu Au;Ge;Ni ð5Þ where iLu
Au;Ge;Ni¼ aiþ biT, and ai and bi are model
parameters to be evaluated in the present optimization. Intermetallic compounds
There are no intermetallic compounds in the Au–Ge and Au–Ni binary systems. In the Ge–Ni binary system, bNi3Ge phase has the ordered variant of the disordered fcc
structure (L12 type). Hence, it was modeled as (Au,Ge,
Ni)0.75(Au,Ge,Ni)0.25in the Au–Ge–Ni ternary system. The
parameters which were introduced by employing Au into the sublattice were given as zero because neither experi-mental nor theoretical thermodynamic data for those metastable end members are available. According to the present experimental results, the solubility of the element Au in the binary Ge–Ni intermetallic compounds is fairly small. Therefore, the Gibbs energies of all the other binary Ge–Ni intermetallic compounds were taken directly from Ref. .
Results and discussion Experimental results
All prepared and investigated samples are listed in Tables1 and2. The microstructures of the samples after heat treatment at 600 °C are shown in Fig.1. The phase compositions were determined by electron probe micro-analysis (EPMA). A two-phase equilibrium between fcc(Au) and Ni5Ge3was observed in alloys 5, 13, and 14
(Table2). Figure1a shows the backscattered electron (BSE) image of annealed sample 5. The compositions of
the dark phase and the white phase as measured by EPMA are 38.7 at.% Ge–61.3 at.% Ni and 97.6 at.% Au–2.4 at.% Ni, corresponding to the Ni5Ge3 and fcc(Au) phases,
respectively. The solubility of Au in the Ni5Ge3 phase is
almost zero. The microstructure of alloy 6 after heat treatment at 600°C for 1,464 h is shown in Fig.1b. The white phase and the big dark phase were identified by EPMA as fcc(Au) and bNi3Ge, respectively. The small
round gray phase is too small to be precisely identified by EPMA. A two-phase microstructure fcc(Au) ? bNi3Ge
was found in alloys 7 and 8 according to their compositions measured by EPMA. Figure1c presents the scanning electron microscopy (SEM) image of annealed alloy 8. Alloy samples 9, 10, 11, and 12 show a two-phase equi-librium between fcc(Au) and fcc(Ni). As an example, the microstructure of annealed alloy 11 is presented in Fig.1d. Table2 lists the compositions of the coexisting phases measured by EPMA on the samples annealed at 600°C. No solubility of Au was detected in the Ni5Ge3phase and the
solubility of Au in bNi3Ge is less than 4 at.%. The
solu-bilities of Ni in fcc(Au) range from 1 to 5 at.% in alloy samples 5, 6, 13, and 14, whereas larger amounts of Ni, from 14 up to 25 at.%, are dissolved in fcc(Au) in samples 7, 8, 9, 10, 11, and 12.
To further confirm the phase constitution, XRD was performed on alloy samples 6, 7, 8, and 10. A three-phase equilibrium, fcc(Au), bNi3Ge, and Ni5Ge3, was confirmed
in annealed alloy 6. The diffraction pattern of the annealed alloy 6 is illustrated in Fig.2a. Combining with the EPMA results, the small round gray phase presented in the annealed microstructure of alloy 6 (Fig.1b) is the Ni5Ge3
phase. Two phases, fcc(Au) and bNi3Ge, were detected in
alloy samples 7 and 8. Figure2b presents the diffraction pattern of the annealed alloy 8. The two-phase equilibrium, fcc(Au) and fcc(Ni), was identified in the annealed alloy 10.
DSC measurements were carried out on samples that had been annealed at 325°C for 648 h. Temperatures of thermal effects which were found in both heating cycles were in good agreement with each other. As significant supercooling was noticed in the recorded cooling curves, relevant phase diagram information was taken from the heating curve. Table1 summarizes the results of the ther-mal analysis from the first heating curve for 10 and 5°C/ min scanning rates. For illustration, Fig.3depicts heating curves obtained by DSC for selected alloy samples.
The microstructures of the as-cast alloys and the alloys after DSC measurements (scanning rate 10°C/min) were
Table 1 Nominal compositions of the Au–Ge–Ni alloys produced by arc-melting, primary phases observed on solidification, phase transfor-mation temperatures measured by DSC during heating
Alloy number Nominal composition/at.% Primary phase DSC signals on heating/°C
Au Ge Ni 5°C/min 10°C/min 1 71.3 27.7 1.0 NiGe 364a 378 386b 362a 375 383b 2 68.4 26.6 5.0 NiGe 363a 464 620b 362a 625b 3 64.1 24.9 11 Ni5Ge3 364a 550a 559c 807b 362a 548a 804b 4 60 23 17 Ni5Ge3 363a 551a 650c 878b 362a 546a 651c 882b 5 50.4 19.6 30 Ni5Ge3 611 832 974b 610 828 970b 6 41.8 16.2 42 bNi3Ge 904a 978b 904a 976b 7 36 14 50 bNi3Ge 931 935c 1,008b 930 937c 1,003b 8 28.8 11.2 60 bNi3Ge 922a 1,040b 921a 1,042b 9 25.2 9.8 65 fcc(Ni) 922a 929c 1,121b 920a 930c 1,122b 10 21.6 8.4 70 fcc(Ni) 922a 924c 931c 1,156b 921a 924c 933c 1,161b 11 14.4 5.6 80 fcc(Ni) 941a 1,278b 941a 1,275b 12 7.2 2.8 90 fcc(Ni) – – – – 1,189 13 74 10.3 15.7 fcc(Au) 871 869 910b 14 68.9 12.3 18.8 Ni5Ge3 896b 899b 15 61 3.2 35.8 fcc(Au) 922a 944b 919a 937b 16 10 80 10 (Ge) 362a 716 854b 362a 718 855b 17 20 60 20 NiGe 363a 702 752b 362a 706 754b
DSC differential scanning calorimetry, – experiment not performed
a Invariant reaction b Liquidus temperature c Weak signal
characterized by SEM, as shown in Figs.4 and 5. Fig-ure4a illustrates the microstructure of the as-cast sample 1. Three phases, fcc(Au), NiGe, and (Ge), were observed, with NiGe as the primary phase. The primary solidification of the Ni5Ge3phase is observed in alloys 3, 4, 5, and 14, as
shown in Fig.4b (alloy 3). The bNi3Ge phase was found as
the primary phase in samples 6, 7, and 8 (Fig.4c, as-cast alloy 6; Fig.4d, as-cast alloy 8). The fcc(Ni) phase was the primary phase in as-cast samples 9, 10, 11, and 12, whereas fcc(Au) was the primary phase in samples 13 and 15. Figure5a, b shows the microstructures of samples 16 and 17 after DSC measurements with the scanning rate of 10°C/min. As can been seen, a three-phase microstructure fcc(Au), (Ge), and NiGe was observed in both samples. However, they show different solidification sequences. The (Ge) phase is the primary phase in sample 16 whereas NiGe crystallized first from the liquid in sample 17. Table1 compiles the primary phases observed in all the alloy samples.
Combining the previous assessments of the Au–Ge , Au–Ni , and Ge–Ni  binary systems, we optimized the Au–Ge–Ni ternary system on the basis of the experi-mental data obtained in the present work. The optimization of the model parameters for various phases in the Au–Ge–
Ni ternary system was conducted using the PARROT module  in the Thermo-calc software package devel-oped by Sundman et al. . The thermodynamic parameters for all condensed phases in the Au–Ge–Ni ternary system obtained in the present work together with the thermodynamic parameters of the three binary systems Au–Ge, Au–Ni, and Ge–Ni from literature [18–20] are summarized in Table 3.
Figure6 shows the calculated isothermal section at 600 °C. Tie-lines determined by EPMA in the present work were superimposed for comparison. The three-phase field fcc(Au) ? Ni5Ge3? bNi3Ge and two-phase fields
fcc(Au) ? Ni5Ge3, fcc(Au) ? bNi3Ge, fcc(Au) ? fcc(Ni)
are well reproduced. However, the nominal composition of alloy 8 lies in a three-phase field fcc(Au) ? bNi
3-Ge ? fcc(Ni) according to the calculation, whereas only two phases fcc(Au) and bNi3Ge were identified in the
annealed sample. It should be noted that similar morphol-ogies were observed for the as-cast state and after annealing, as can been seen from Figs. 1c and 4d. This implies that full equilibrium has possibly not been obtained in alloy 8. Besides, the calculated solubilities of Au and Ge in fcc(Ni) are lower than the measured values. The dif-ference may be due to full equilibrium not being achieved in alloys 9, 10, 11, 12 even after 1,462 h of annealing. This can be seen from the BSE image of annealed alloy 11 (Fig.1d) in which the fcc(Ni) phase appears in different
Table 2 Summary of the phase compositions measured by EPMA for the Au–Ge–Ni ternary alloys annealed at 600°C
ND not possible to determine, XRD X-ray diffraction
Alloy number Annealing time/h EPMA results/at.% Phase identified Technique
Au Ge Ni 5 720 0 38.7 61.3 Ni5Ge3 EPMA 97.6 0 2.4 fcc(Au) EPMA 6 1,464 3.3 23.7 73 bNi3Ge EPMA ? XRD 94.7 0 5.3 fcc(Au) EPMA ? XRD ND ND ND Ni5Ge3 XRD 7 1,464 1.1 24 74.9 bNi3Ge EPMA ? XRD 86.3 0 13.7 fcc(Au) EPMA ? XRD 8 1,464 4 21 75 bNi3Ge EPMA ? XRD 84 0 16 fcc(Au) EPMA ? XRD 9 1,464 4.6 11.4 84 fcc(Ni) EPMA 79 0 21 fcc(Au) EPMA 10 1,464 5.1 9.4 85.6 fcc(Ni) EPMA ? XRD 79 0 21 fcc(Au) EPMA ? XRD 11 1,464 5.2 6.1 88.7 fcc(Ni) EPMA 76 0 24 fcc(Au) EPMA 12 1,464 3.3 2.6 94 fcc(Ni) EPMA 75 0 25 fcc(Au) EPMA 13 720 0 38.1 61.9 Ni5Ge3 EPMA 95 0 5 fcc(Au) EPMA 14 1,464 0 38.7 61.3 Ni5Ge3 EPMA 98.8 0 1.2 fcc(Au) EPMA
contrasts, which means that interdiffusion of the elements is still going on.
The calculated vertical section Au72Ge28–Ni compared
with the experimental data obtained in the present work is shown in Fig.7. Good agreement between calculation and experiment was obtained. The liquidus and most of the phase transformations were well reproduced. However, there are some deviations for alloy 1. Three thermal signals were observed in alloy 1. The first thermal effect was measured at T = 363°C (the average value of the data at 5 and 10 °C/ min), agreeing well with the calculated value 357°C. The second thermal effect happened at T = 378°C while the calculated temperature is 406°C. The difference originates from the deviation of the calculated eutectic composition from the experiment in the Au–Ge binary system. The investigated vertical section in this work starts from the Au– Ge experimental eutectic point (28 at.% Ge) to pure Ni. However, the calculated Au–Ge eutectic composition is at
29.5 at.% Ge , which leads to the higher calculated transition temperature for the Au–Ge–Ni ternary alloy 1. The calculated liquidus temperature (ca. 460°C) for alloy 1 is also higher than the corresponding experimental value (386 °C). If the liquidus temperatures of alloy 1 and all the other alloys were reproduced at the same time, the liquidus would have to be much steeper in a very narrow composition range, from 0 to 4 at.% Ni, which is unreasonable. Hence, the measured liquidus temperature of alloy 1 might have large experimental uncertainty, which may arise from the inhomogeneity of the sample.
Besides, the thermal signals for the phase transforma-tions at low temperature in alloy 6, 7, 8, and 9 were not observed or were too weak to be analyzed. It should be noted that there is no liquid phase involved in those reac-tions. The liquidus temperature of alloy 12 was not reached because the maximum measuring temperature was 1,300°C.
Fig. 1 BSE images of the Au–Ge–Ni alloy samples annealed at 600°C. a Alloy 5: Au–19.6 at.% Ge–30 at.% Ni, b alloy 6: Au–16.24 at.% Ge–42 at.% Ni, c alloy 8: Au–11.2 at.% Ge–60 at.% Ni, d alloy 11: Au–5.6 at.% Ge–80 at.% Ni
Figure8 shows the calculated vertical section at Ge– Au50Ni50compared with the experimental data obtained in
the present work. As can be seen, good agreement was obtained.
The calculated liquidus projection of the Au–Ge–Ni ternary system superimposed with the experimentally determined primary phases is presented in Fig.9. The regions of primary crystallized phases observed in the present work are generally well reproduced in the present calculation, but some discrepancies were found in alloys 2, 8, and 14. It should be noted that the nominal com-positions of those alloys are very close to the monovariant line.
Table4 summarizes the types and temperatures of the invariant reactions together with the compositions of the participating liquid phases. The invariant reactions U1
(L ? cNi3Ge $ bNi3Ge ? dNi5Ge2) and U2 (L ? dNi
5-Ge2$ Ni5Ge3? bNi3Ge) were not investigated
experimentally in the present work due to the too small primary crystallization fields of cNi3Ge and dNi5Ge2. An
interesting ternary quasi-peritectic U3 (L ? fcc$ fcc ?
bNi3Ge) at 937°C is predicted by the present calculation.
The existence of this ternary quasi-peritectic invariant reaction (U3) was proved by the experimental results. As can
be seen from Table 1, a ternary invariant reaction which happens at 921°C was observed in alloys 8, 9, 10, and 15. The ternary eutectic reaction E1(L$ Ge ? NiGe ? fcc)
and ternary quasi-peritectic reaction U4 (L ? bNi3Ge$
fcc ? Ni5Ge3) are well reproduced, with only a temperature
difference of 5 and 15°C between calculation and experi-ment, respectively. However, for the reaction U5
(L ? Ni5Ge3$ NiGe ? fcc), the calculated invariant
temperature is 497 °C, 52 °C lower than the corresponding experimental value (549 °C). This difference is caused by the thermodynamic parameters of the NiGe phase in the Ge–Ni binary system. The temperature difference could be shortened and meanwhile the nominal composition of alloy 2 would fall into the NiGe primary crystallization field if a more exothermic enthalpy of formation for the NiGe phase was given. However, the reaction type of the binary invariant reaction Ni5Ge3$ e0Ni5Ge3? NiGe will be changed from
eutectoid to peritectoid (Ni5Ge3? NiGe$ e0Ni5Ge3) in
the Ge–Ni binary system. Besides, a temperature difference of 50 °C is considered to be still acceptable for this ternary system. Therefore, the thermodynamic parameters of the NiGe phase are kept the same as the one from the binary system .
The ternary eutectic temperature of 425°C which was quoted by Christou  was not found in the present work. However, Christou  only mentioned that it was deter-mined by a resistivity technique. No further details were given in his work.
A detailed overview over the nature and sequence of these ternary invariant reactions and their connections to the binary boundary systems is given by the calcu-lated reaction scheme (Scheil diagram) shown in Fig.10.
Fig. 2 Diffraction patterns of the samples after heat treatment at 600°C. a Alloy 6: Au–16.24 at.% Ge–42 at.% Ni, b alloy 8: Au– 11.2 at.% Ge–60 at.% Ni
Fig. 3 DSC curves recorded upon heating with a rate of 10°C/min for selected samples
Fig. 4 As-cast microstructures of a alloy 1: Au–27.72 at.% Ge–1 at.% Ni, b alloy 3: Au–24.92 at.% Ge–11 at.% Ni, c alloy 6: Au–16.24 at.% Ge–42 at.% Ni, d alloy 8: Au–11.2 at.% Ge–60 at.% Ni
Fig. 5 Microstructures of the samples after DSC measurement (scanning rate 10°C/min). a Alloy 16: Au–80 at.% Ge–10 at.% Ni, b alloy 17: Au–60 at.% Ge–20 at.% Ni
Table 3 Thermodynamic parameters of the Au–Ge–Ni ternary system
Gibbs energies are expressed in J/mol. The lattice stabilities were given by Dinsdale  References Liquid (Au,Ge,Ni) 0Lliquid Au;Ge¼ 18; 294:684 13:671T  1Lliquid Au;Ge¼ 8; 894:639 6:339T  2Lliquid Au;Ge¼ 2; 174:476 4:925T  0Lliquid Au;Ni¼ 9; 500 5:429T  1Lliquid Au;Ni¼ 1; 614  0Lliquid Ge;Ni¼ 167; 121:320 þ 155T 15T ln T  1Lliquid Ge;Ni¼ 84; 737:489 25:014T  2Lliquid Ge;Ni¼ 37; 441:590 16:001T  3Lliquid Ge;Ni¼ 63; 650:323 þ 21:983T  0Lliquid
Au;Ge;Ni¼ 140; 000 This work
fcc: (Au,Ge,Ni) 0Lfcc Au;Ge¼ 10; 198:859 23:114T  0Lfcc Au;Ni¼ 28; 696 11:274T  1Lfcc Au;Ni¼ 10; 945 þ 6:154T  2Lfcc Au;Ni¼ 2; 519  0Lfcc Ge;Ni¼ 122; 000 þ 36:88T  1Lfcc Ge;Ni¼ 134; 000 46:8T  0Tcfcc Ge;Ni¼ 3; 750  0Lfcc
Au;Ge;Ni¼ 320; 000 This work
Au;Ge;Ni¼ 0 This work
Au;Ge;Ni¼ 91; 000 This work
0GbNi3Ge Ge:Ni 0:750GdiamondGe 0:250GfccNi ¼ 46; 827:192 þ 3:05T  0GbNi3Ge Ni:Ge 0:250GdiamondGe 0:750GfccNi ¼ 46; 827:192 þ 3:05T  0GbNi3Ge Ge:Ge 0GdiamondGe ¼ 0  0GbNi3Ge Ni:Ni 0GfccNi ¼ 0  0LbNi3Ge Ge;Ni:Ge¼ 93; 654:384 þ 6:1T  0LbNi3Ge Ge;Ni:Ni¼ 93; 654:384 þ 6:1T  1LbNi3Ge Ge;Ni:Ge¼ 23; 700 9:72T  1LbNi3Ge Ge;Ni:Ni¼ 23; 700 9:72T  0LbNi3Ge Ni:Ge;Ni¼ 0  0LbNi3Ge Ni:GeGe¼ 0  1LbNi3Ge Ni:Ge;Ni¼ 7; 900 3:24T  1LbNi3Ge Ge:Ge;Ni¼ 7; 900 3:24T 
Ni:Ge 0:2560GdiamondGe 0:7440GfccNi ¼ 34; 315 þ 4:301T 
Ni:Ge 0:280GdiamondGe 0:720GfccNi ¼ 34; 918 þ 3:69T 
0GNi2Ge Ni:Ge 0:3350GdiamondGe 0:6650GfccNi ¼ 38; 227:151 þ 4:849T  Ni5Ge3: (Ge)(Ni)(Va,Ni) 0GNi5Ge3 Ge:Ni:Va0GdiamondGe 0GfccNi ¼ 54; 286:304 5:624T  0GNi5Ge3 Ge:Ni:Ni0GdiamondGe 20GfccNi ¼ 110; 540 þ 11:717T  0LNi5Ge3 Ge:Ni:Ni;Va¼ 2; 655:913 2:932T  1LNi5Ge3 Ge:Ni:Ni;Va¼ 17; 558:144 
Ni:Ge 0:3750GdiamondGe 0:6250GfccNi ¼ 37; 350:646 þ 3:328T 
Ni:Ge 0:50GdiamondGe 0:50GfccNi
¼ 30; 992:547 þ 0:967T 0:1T ln T þ 6:015E 05T2
9:471E 08T3þ 2:393E 22T7 14; 960:491T1
Phase equilibria in the Au–Ge–Ni ternary system were experimentally studied and a full thermodynamic descrip-tion was established. A vertical secdescrip-tion at Au72Ge28–Ni and
a partial isothermal section at 600°C were experimentally determined. The solubility of Au in the Ni5Ge3 phase is
less than 4 at.% and no solubility of Au was observed in the bNi3Ge phase. No ternary compound was found at
600 °C. The calculated liquidus projection reproduces the experimental data well. Five ternary quasi-peritectic reac-tions and one ternary eutectic reaction were proposed. The reasonable agreement between the thermodynamic calcu-lations and the experimental results supports the reliability of the present thermodynamic modeling of the Au–Ge–Ni ternary system. These results provide important informa-tion for developing and designing Au–Ge-based alloys as high-temperature lead-free solders.
Seventeen samples with different composition were pro-duced. All alloy compositions are listed in Table1. The starting materials were pure elements of Au wire (99.99 %), Ge pieces (99.999 %), and Ni slug and wire (99.98 %) supplied by Alfa Aesar GmbH, Germany.
Alloys of 1 g were produced by arc-melting under high-purity argon atmosphere (Ar 6.0) using a non-consumable tungsten electrode. All alloys were melted five times and inverted after three meltings to ensure homogeneity. In order to have a clean atmosphere during the melting, a Ti alloy was melted first as an oxygen getter. In addition, an oxygen cartridge in the argon line was used. No chemical analysis of the alloys was conducted because the weight losses during melting were less than 0.3 mass% in all cases.
Afterwards, the samples were cut into three pieces for different purposes. One was used to investigate the as-cast
Fig. 6 Calculated isothermal section at 600°C compared with the experimental data measured in the present work
Fig. 7 Calculated vertical section at Au72Ge28–Ni compared with the
microstructure; another one was used for DSC measure-ments after homogenization heat treatment at 325°C for 648 h; and one was used to investigate the microstructure after annealing experiments at 600°C. For the heat treat-ments the samples were placed in evacuated quartz tubes refilled with argon. Before the encapsulation the samples were cleaned in acetone, dried, and wrapped in tantalum foil to avoid reactions with the quartz tube. The annealing
experiments were performed at 600°C for 720–1,464 h in an electric resistance furnace with a temperature accuracy of ±3°C. After annealing, the samples were quenched in salt water to retain the equilibrium microstructures.
Phase transitions and thermal reactions were determined by DSC performed on a Netzsch DSC 404 F3 Pegasus, using open alumina crucibles. The DSC cells were cali-brated using the melting temperatures of the pure elements
Fig. 8 Calculated vertical section at Ge–Au50Ni50
compared with the experimental data in the present work
Fig. 9 Calculated liquidus projection of the Au–Ge–Ni ternary system superimposed with the experimental data of primary solidification
Sn, Bi, Al, In, Ag, and Au. Samples after homogenization heat treatment at 325°C for 648 h were used in the DSC experiments. The samples were polished and cleaned just before being measured in order to improve thermal contact and to avoid spurious or shifted transition peaks due to oxidation. Before each experiment, the DSC cell was evacuated three times and refilled with high-purity argon. Measurements were performed under a continuous flow of argon at a scanning rate of 10°C/min (heating and cooling) and 5°C/min (heating and cooling), separately. For each sample two heating/cooling cycles were performed.
The as-cast samples, annealed samples, and the samples after DSC measurements were then examined by SEM, XRD, and EPMA. XRD measurements were performed on a Panalytical X’Pert Pro X-ray diffractometer using
Cu-Ka1 radiation (40 kV, 40 mA) filtered with a
Ge(111)-crystal monochromator at room temperature. The scanning range was 10° \ 2h \ 100° with a step size of 0.017° and a scan speed of 0.027°/s.
The compositions of the coexisting phases of each sample were determined by EPMA using a JEOL JXA8800 microanalyzer with an acceleration voltage of 30 kV and a probe current of 4 9 10-8A. Pure element standards provided by JEOL were used for calibration. The mea-surements have a relative accuracy of about 1 %.
Acknowledgments This work was financially supported by the Swiss State Secretariat for Education and Research (SBF No. C08.0031) within the European COST action MP0602 on high tem-perature lead-free solder materials as well as by the Swiss National Science Foundation (SNSF no. 200021_134575/1).
Table 4 Calculated ternary invariant reactions involving liquid phase with the experimental data
Invariant reaction Type T/°C Composition in liquid (calculation)
Experiment Calculation Au/at.% Ge/at.% Ni/at.%
L ? cNi3Ge$ bNi3Ge ? dNi5Ge2 U1 – 1,102 0.6 28.9 70.5
L ? dNi5Ge2$ Ni5Ge3? bNi3Ge U2 – 1,097 1.3 28.8 69.9
L ? fcc$ fcc ? bNi3Ge U3 921 937 43 8.7 48.3
L ? bNi3Ge$ fcc ? Ni5Ge3 U4 904 889 55.7 15.2 29.1
L ? Ni5Ge3$ NiGe ? fcc U5 549 497 74.5 24.0 1.5
L$ Ge ? NiGe ? fcc E1 362 357 70.2 29.6 0.2
Fig. 10 Reaction scheme of the Au–Ge–Ni ternary system
1. Kang N, Na HS, Kim SJ, Kang CY (2009) J Alloy Compd 467:246
2. Kim SJ, Kim K-S, Kim S-S, Suganuma K (2009) J Electron Mater 38:266
3. Fima P, Gasior W, Sypien A, Moser Z (2010) J Mater Sci 45:4339
4. Schoeller H, Bansal S, Knobloch A, Shaddock D, Cho J (2009) J Electron Mater 38:802
5. Park J-H, Lee J-H, Kim Y-S (2002) J Electron Mater 31:1175 6. Toshio T, Satoru K, Masanori K, Noriharu K, Katsuhiko S (2005)
Mater Trans 46:1825
7. Wang Q, Choa S-H, Kim W, Hwang J, Ham S, Moon C (2006) J Electron Mater 35:425
8. Massalski B (1990) Binary alloy phase diagrams. ASM, Metals Park
9. Chidambaram V, Hald J, Hattel J (2009) Microelectron Reliab 49:323
10. Chidambaram V, Hald J, Hattel J (2010) J Alloy Compd 490:170 11. Leinenbach C, Valenza F, Giuranno D, Elsener HR, Jin S,
No-vakovic R (2011) J Electron Mater 40:1533
12. Lang FQ, Yamaguchi H, Ohashi H, Sato H (2011) J Electron Mater 40:1563
13. Rai AK, Bhattacharya RS, Park YS (1984) Thin Solid Films 114:379
14. Piotrowska A, Guivarch A, Pelous G (1983) Solid State Electron 26:179
15. Jaffee RI, Gonser BW (1946) Trans Am Inst Min Met Eng 166:436
16. Christou A (1979) Solid State Electron 22:141
17. Kaufman L, Bernstein H (1970) Computer calculation of phase diagrams. Academic, New York
18. Wang J, Leinenbach C, Roth M (2009) J Alloy Compd 48:1830 19. Wang JH, Lu X-G, Sundman B, Su XP (2005) CALPHAD
20. Jin S, Leinenbach C, Wang J, Duarte LI, Delsante S, Borzone G, Scott A, Watson A (2012) CALPHAD (accepted)
21. Dinsdale AT (1991) CALPHAD 15:317
22. Redlich O, Kister AT (1948) Ind Eng Chem 40:345
23. Jansson B (1984) Tricta-Mac-0234. Royal Institute of Technol-ogy, Stockholm